21Electrically Conductive Adhesives
Johann Nicolics and Martin Miindlein
Institute ofSensor and Actuator Systems, Gusshausstraj3e 27-29, A-I040 Wien, Austria
Abstract Electrically conductive adhesives are being used in electronic packaging for severaldecades. A brief review of the dynamic development of conductive adhesives under theinfluence of the miniaturization, the adaptation of environmental friendly manufactur-ing processes is presented.With respect to the importance of isotropically conductive adhesives (ICA), a new con-tact model to analyze the principle influences of e.g., particle size, particle geome-try, and filler content on the percolation threshold is introduced. With this model thearrangement of the particles within a contact is calculated by considering differenttypes of forces (elastic, friction, adhesion, and inertia). Taking into account the electri-cal properties of the filler particles, the electrical contact behavior including its changesdue to aging is investigated.Finally, typical applications of isotropically conductive adhesives are presented. Oneexample shows how the thermal requirements for attaching a GaAs heterojunctionpower transistor can be fulfilled using an adhesive with an extremely high filler content(thermal conductivity: >60 W/mK). In another case it is demonstrated how extremethermomechanical requirements resulting from a thermal expansion mismatch of partsof a sealed IR sensor housing can be corresponded using an adhesive with a compara-tively low glass transition temperature. A further example shows a packaging concept ofa miniaturized, biocompatible multichip module. For mounting both. narrowly spacedSMDs and bare chips. an isotropically conductive adhesive has been applied.
21.1. INTRODUCTION AND HISTORICAL BACKGROUND
The industrial application of electrically conductive adhesives (ECA) for intercon-necting and mounting electronic components on circuit carriers is comparatively new. How-ever, a series of inventions related to various mixtures of conductive and non-conductivesubstances were made already in the first half of the last century. An early patent of an elec-trically conductive adhesive describes electromechanical applications already in 1926 .In 1933 Hans Schuhmann claims a conducting varnish (consisting of a mixture of about50% oil varnish, about 40% lithopone, and 10% of soot) which can be applied for shieldingpurposes in the radio industry . Only two years later it turned out that conducting layersconsisting of a binding agent mixed with a finely divided conductor lose their conductivityduring operation or do not at all posses this conductivity even if applied in the form in
572 JOHANN NICOLICS AND MARTIN MUNDLEIN
which they are on the market . In 1944 H.J. Loftis proposed a molded electrically con-ductive body consisting of Bakelite as the resin filled with graphite or metal powder and anadditive of an alkaline earth metal salt providing hygroscopic properties to preserve a lu-bricating effect for the use as commutator brush . An early description of an electricallyconductive adhesive more similar to the modem ECA can be found in the patent of N.H.Collings et II. in 1948 on the base of a self-setting adhesive and, e.g., finely divided silverpowder .
The first use of ECAs in electronic technology is known only in 1956: in the U.S.patent  an electrically conducting cement comprising a thermosetting binding mediumis desclibed for fixing a semi-conducting clystal (germanium) to a metal base or holder.Thereafter, the number of publications reporting experimental and theoretical investi-gations of electrically conductive adhesives increased continuously. Twenty years laterC. Mitchel and H. Berg summmized the state-of-the-mt in 1976. They reported that con-ductive adhesives due to their increasing reliability become more and more acceptable formany different applications. Also the most significant advantages compared to other inter-connection techniques, such as low processing temperature and the possibility to use a largevariety oflow-cost sUIface fillers are already mentioned . Especially for mounting chipswith larger size on substrates with different coefficient of thermal expansion adhesives aresuperior to eutectic solder alloys due to their significantly higher flexibility. Conductiveadhesive bonding started to become populm' with the fabrication of plastic-foil keyboardsand the use of flexible substrate materials .
More recently, in 2000, Alan J. Heeger, Alan G. MacDiarmid and Hideki Shirakawaare awarded the Nobel Prize in Chemistry for their discovery of electrically-conductingpolymers whereby initial experiments with silvery shining films of polyacetylene lead backto the beginning of the 1970s .
Along with the development of liquid crystal displays (LCDs) in the 80s and theircontinuing miniaturization a special kind of ECA-the anisotropic conductive adhesive(ACA) has been invented for components with high-lead count and fine pitch interconnec-tions [10,11]. ACAs allow to produce an excellent low-ohmic contact only perpendicularto the mating metalization planes whereby one-particle contact bridges between these met-alizations are formed. However, due to their very low loading of conductive filler particles,ACAs remain insulating in the lateral direction. As such, no high-precision printing processis needed. In the meanwhile, ACAs are successfully applied especially for high-resolutiondisplays in portable devices such as notebooks and PDAs (Personal Digital Assistant). Al-though, the capability of ACAs for comparatively high current load with even up to severalAmperes per square millimeter were investigated , due to their low filler content theirmain application fields will probably remain the interconnection of components with lowCUlTent consumption.
Whereas ACAs have a volume resistivity like an insulator, another type of ECA witha significantly higher degree of conductive filler has a low volume resistivity, compara-ble with that of conductors (Figure 21.1). They are called isotropic conductive adhesives(ICA, ). The goal of this chapter is to develop a deeper understanding of the contact for-mation process and the influence of application related parameters on the electrical contactresistance of ICAs.
The ICA technology became more interesting in the last years due to several reasons.One of the major driving forces is the increasing packaging density allowing to develop ahuge manifold of complex but nevertheless light portable electronic equipments like e.g.,cell phones, digital cameras, and notebooks. This development was mainly based on threekey factors:
ELECTRICALLY CONDUCTNE ADHESIVES
FIGURE 21.1. SEM cross-sectional view of an ICA.
an inconceivable fineness of structures in the semiconductor level coming close to0.1 flm and allowing a high integration level,a decrease of package size coming down from small outlined (SO) packages overquad flat pack (QFPs), ball-grid alTays (BGAs), and chip-scale packages (CSPs) todirect or bare chip attach techniques like flip-chips (FCs), andnew printed circuit board manufacturing (PCB) techniques like microvia multilayertechnology with plasma or laser structured vias with even less than 0.1 mm diameterallowing to realize a three-dimensional wiring net with extremely high density.
Although, soldering technology has matured through many decades, with the men-tioned advances in microelectronics technology a limitation of solder paste become moreand more evident in its use for fine pitch components . With CUlTent solder paste tech-nology very fine pitch interconnection become hard to handle due to soldering defects suchas bridging and solder balling [15-17]. This means to connect the components on the circuitboards under these boundary conditions improved or new interconnection technologies areneeded. One of these new techniques could be conductive adhesive bonding. Among thesetechnical demands new legislative reforms make an adaptation of the existing technologiesnecessary. From the 1st July 2006 on member states of the European Union have to ensurethat new electrical and electronic equipment does not contain lead, mercury, cadmium andother named materials. This is regulated in the directive 2002/95JEC of the European Par-liament and of the Council on the restriction of the use of certain hazardous substances inelectrical and electronic equipment . Under these restriction the prohibition oflead ismost serious for the packaging technology because the widely applied solder technologycommonly uses solder pastes consisting of a tin lead alloy.
Due to their composition conductive adhesives are innately lead free. Additionally,they allow to avoid flux residues without cleaning. They need a low processing temper-ature but allow operation at high temperatures. Adhesives are preferable whenever highelasticity is needed to compensate for thermal expansion mismatch between substrate andcomponent body [19-22]. However, compared to soldering, electrically conductive adhe-sive technology is still in its infancy [23,24]. Two critical issues of conductive adhesives for
574 JOHANN NICOLICS AND MARTIN MUNDLEIN
surface mount applications are the contact resistance shift during lifetime and a low impactperformance . As a long-term effect, the contact resistance of ECAs on ignoble metalfinishes can increase dramatically during exposure to elevated temperature and humidity.The low impact performance is observed by separation of components from the board dueto impact of significant shock during manufacturing and lifetime of the product. The abilityof ECAs to withstand this stress can be determined with the standardized drop test .Another drawback of one-component adhesives compared to soldering is also frequentlycited: a lo